The volume of an electrolytic capacitor is defined by the product of capacitance and voltage, the so-called CV-volume. However, in comparing the permittivities of different oxide materials, it is seen that tantalum pentoxide has an approximately 3 times higher permittivity than aluminum oxide. Tantalum electrolytic capacitors of a given CV value can therefore be smaller than aluminum electrolytic capacitors. Basic construction of solid tantalum electrolytic capacitors A typical tantalum capacitor is a chip capacitor and consists of tantalum powder pressed and sintered into a pellet as the anode of the capacitor, with the oxide layer of tantalum pentoxide as a dielectric, and a solid manganese dioxide electrolyte as the cathode. Materials, production and styles Anode Tantalum capacitors are manufactured from a powder of relatively pure elemental tantalum metal. A common figure of merit for comparing volumetric efficiency of powders is expressed in capacitance (C, usually in μF) times volts (V) per gram (g). Since the mid-1980s, manufactured tantalum powders have exhibited around a ten-fold improvement in CV/g values (from approximately 20k to 200k). The typical particle size is between 2 and 10 μm. Figure 1 shows powders of successively finer grain, resulting in greater surface area per unit volume. Note the very great difference in particle size between the powders. The powder is compressed around a tantalum wire (known as the riser wire) to form a "pellet". The riser wire ultimately becomes the anode connection to the capacitor. This pellet/wire combination is subsequently vacuum sintered at high temperature (typically 1200 to 1800 °C) which produces a mechanically strong pellet and drives off many impurities within the powder. During sintering, the powder takes on a sponge-like structure, with all the particles interconnected into a monolithic spatial lattice. This structure is of predictable mechanical strength and density, but is also highly porous, producing a large internal surface area (see Figure 2). Larger surface areas produce higher capacitance; thus high CV/g powders, which have lower average particle sizes, are used for low voltage, high capacitance parts. By choosing the correct powder type and sintering temperature, a specific capacitance or voltage rating can be achieved. For example, a 220 μF 6 V capacitor will have a surface area close to 346 cm2, or 80% of the size of a sheet of paper (US Letter, 8.5×11 inch paper has area ~413 cm2), although the total volume of the pellet is only about 0.0016 cm3. Dielectric